Research Article www.acsami.org
Facile in Situ Synthesis of Silver Nanoparticles on ProcyanidinGrafted Eggshell Membrane and Their Catalytic Properties Miao Liang,† Rongxin Su,*,†,§ Renliang Huang,‡ Wei Qi,†,§ Yanjun Yu,† Libing Wang,† and Zhimin He† †
State Key Laboratory of Chemical Engineering, School of Chemical Engineering and Technology, Tianjin University, Tianjin 300072, P. R. China ‡ School of Environmental Science and Engineering, Tianjin University, Tianjin 300072, P. R. China § Collaborative Innovation Center of Chemical Science and Engineering (Tianjin), Tianjin 300072, P. R. China S Supporting Information *
ABSTRACT: Facile, eﬃcient, and robust immobilization of metal nanostructures on porous bioscaﬀolds is an interesting topic in materials chemistry and heterogeneous catalysis. This study reports a facile in situ method for the synthesis and immobilization of small silver nanoparticles (AgNPs) at room temperature on natural eggshell membrane (ESM), which presents interwoven ﬁbrous structure and can be used as a unique protein-based biotemplate. Procyanidin (Pro), a typical plant polyphenol extracted from grape seeds and skins, was ﬁrst grafted onto ESM ﬁbers to serve as both reductant and stabilizer during the synthesis process. As a result, the AgNPs were facilely synthesized and robustly immobilized on the ESM ﬁbers without additional chemical reductant or physical treatments. The morphology and microstructure of the as-prepared [email protected]
composites were characterized by combined microscopy and spectroscopy technologies. The results indicate that small AgNPs with mean diameter of 2.46 nm were successfully prepared on the Pro-ESM biotemplate. The composites exhibited good catalytic activity toward the reduction of 4-nitrophenol (4-NP). More importantly, these composite catalysts can be easily recovered and reused for more than eight cycles because of their high stability. KEYWORDS: eggshell membrane, procyanidin, silver nanoparticles, catalysis, 4-nitrophenol
an eﬀective strategy in protecting these metal NPs against agglomeration and facilitating their recovery. Among the various matrixes, macroscopic materials with threedimensional (3D) interconnected porous networks are promising for the immobilization of NPs.11−13 The porous structure endows these supports with high surface area for maximizing NP loading. For instance, Na and co-workers14 have demonstrated that hierarchical carbon nanotube membrane can be used as support for incorporating gold NPs in the catalytic degradation of 4-nitrophenol (4-NP). In addition, polymer hydrogels have also been utilized as matrixes for the incorporation of NPs to combine the catalytic properties of nanocatalyst with the open porous structure and external stimuli-responsive characteristics of hydrogels.15,16 Moreover, the preparation of novel composite catalysts using macroscopic biomaterials with 3D porous
In the ever-expanding ﬁeld of nanomaterials research, noble metal nanoparticles (NPs) (e.g., Au, Ag, Pt) have received considerable attention because of their fascinating physicochemical properties and remarkable potential applications in catalysis, sensing, photonics, and biomedicine.1,2 In particular, the catalytic properties of metallic NPs are appealing to many researchers because of their high reactivity and selectivity.3 The large surface area to volume ratio of NPs contributes to their good catalytic performance. However, nanocatalyst powders are undesirable for industrial applications because of their characteristics, such as easy aggregation, reduction in catalytic activities, and diﬃculty in product separation and catalysts recycling.4−6 Therefore, it is highly desirable to design and synthesize small nanocatalyst with long-term stability for maintaining its catalytic activity during the reactions. Over the past few decades, many eﬀorts have been devoted to developing composite catalysts by immobilizing noble metal NPs on/into solid matrix,7−10 which appears to be © 2014 American Chemical Society
Received: August 20, 2013 Accepted: March 13, 2014 Published: March 13, 2014 4638
dx.doi.org/10.1021/am500665p | ACS Appl. Mater. Interfaces 2014, 6, 4638−4649
ACS Applied Materials & Interfaces
of metallic nanoparticles.31 Additionally, this nontoxic and facile synthesis route is compatible with the sustainable development principles. Given the above merits of ESM and procyanidin, an eﬃcient template was demonstrated for the facile and in situ fabrication of heterogeneous catalysts by grafting procyanidin onto the surface of the ESM ﬁbers. The availability of synthesizing AgNPs using procyanidin was ﬁrst conﬁrmed in aqueous solution. Procyanidin was then covalently grafted onto the ESM ﬁbers through electrophilic agent glutaraldehyde, which provides a novel template for robust immobilization of nanocatalyst. To the best of our knowledge, this study was the ﬁrst to report the in situ and facile synthesis of noble metal NPs on natural ESM using a “green” reductant for catalytic application. Small AgNPs with narrow size distribution were successfully synthesized in situ on the ESM ﬁbers by the reducing and stabilizing ability of procyanidin. The main physical and chemical properties of the as-prepared catalysts were fully characterized. Meanwhile, the catalytic performance of the composite catalysts was investigated by employing the reduction of 4-NP into 4-aminophenol (4-AP) as a model reaction. The elegance of our hybrid system is that the composite catalysts can be easily separated from the reaction mixture after the reaction, allowing the catalysts to be reused without losing their activity signiﬁcantly.
structure has been the focus of numerous studies. For example, Lu and our group have synthesized noble metal nanocatalysts using a chemical reduction or a biomineralization mimetic method in protein crystals that are composed of highly ordered protein assemblies with unique nanosized porous structures.17−19 Fabrication of the above-mentioned macroscopic supports with interconnected pore networks usually involves either high temperature calcination or sophisticated manipulation (polymer cross-linking or protein crystallization), which hinders their extensive applications. Such drawbacks stimulate the exploration of new applicable and cost-eﬀective porous supporting medium with excellent practical utility for nanocatalyst immobilization. Eggshell membrane (ESM), a naturally available protein-based material with interwoven ﬁbrous 3D structure, shows great promise as a novel biotemplate for immobilizing nanocatalysts. Currently, ESM has long been treated as agricultural waste and disposed in landﬁlls without any pretreatment. However, this naturally occurring membrane possesses special characteristics, such as the ability to transport nutrients to the developing embryo and the intricate lattice network of stable protein ﬁbers,20 resulting in high surface area that allows high loading capacity for NPs. In recent years, ﬂuorescent metal nanoclusters and semiconductor NPs have been successfully synthesized and immobilized on this solid matrix mainly through physical interaction.21,22 Actually, the functional properties of these composite systems have seldom been reported, although they oﬀer great potential applications for catalysis, chemical sensing, surface enhanced Raman scattering, and so on. This phenomenon may be caused by the fact that the NPs were physically immobilized on the ESM, and thus, the insuﬃcient stability of NPs limits the practical applications. Our recent work also found that the weak noncovalent interaction between ESM ﬁbers and NPs was not strong enough to maintain the stability and catalytic property of the composites during the recycling process.23 Therefore, chemical modiﬁcation of ESM ﬁbers for improving the stability of supported NPs is desirable in order to realize the practical application of these ESM-based composites. In this study, we prepared a surface modiﬁed and redox-active template, procyanidin-grafted ESM, for robust immobilization of silver nanoparticles (AgNPs). As eﬃcient and cost-eﬀective noble metal nanocatalysts, AgNPs have been applied in various catalytic reactions, such as reduction and oxidation.24−26 The size of AgNP has a signiﬁcant role on catalysis. Smaller AgNPs usually exhibit higher catalytic activity due to their greater surface to volume ratio.6 Thus, developing eﬀective methods for the synthesis of small and well dispersed AgNPs is necessary. Herein, procyanidin has been used, for the ﬁrst time, as both reducing agent and stabilizer for the preparation of small AgNPs with suﬃcient dispersion. Procyanidin, a biologically active polyphenolic ﬂavonoid, is mainly extracted from grape seeds and skins and expected to possess reducing ability toward silver or gold ions.27,28 Previous studies have indicated that the phenolic hydroxyl groups of ﬂavonoid compounds can chelate and reduce silver ions to metallic silver in situ.29,30 Accordingly, procyanidin promises to be an excellent chemical that would be able to synergistically construct a stable linkage between ESM ﬁber and Ag+ ions. Moreover, the utilization of procyanidin avoids the introduction of traditional organic solvents and chemical reductants, such as N,N-dimethylformamide and sodium borohydride, which are highly reactive and pose potential environmental and biological risks. Hence, this natural extracted compound can be accepted as “green” reductant for the synthesis
Materials. Grape-seed-derived procyanidin dimer (≥98%, relative molecular mass of 578.38) was generously provided by JF-Natural (Tianjin, China). Fresh membrane-bound eggshell was collected from a campus breakfast shop and immediately stored in water at 4 °C. Glutaraldehyde (50 wt %), silver nitrate (AgNO3), sodium borohydride (NaBH4), and 4-NP (99%) were purchased from Aladdin Reagent Company (Shanghai, China). Deionized water was used for all the experiments. Synthesis of AgNPs in Aqueous Solution Using Procyanidin. The AgNPs were synthesized using procyanidin as both reducing and stabilizing agent. Procyanidin stock solution (10 mM) was prepared by dissolving a speciﬁc amount of procyanidin powder in deionized water. The stock solution was passed through 0.22 μm sterile ﬁlters to remove foreign nucleation sources before use. In a typical experiment, 6.8 mg of AgNO3 was ﬁrst dissolved in 19 mL of deionized water. Subsequently, 1 mL of procyanidin solution was rapidly added to the precursor solution under continuous stirring. The mixture was allowed to react under continuous magnetic stirring at 310 K. Samples were obtained at diﬀerent reaction times and deposited into a −40 °C deep freeze refrigerator to quench the reaction until further study. Preparation of Procyanidin Grafted Eggshell Membrane (Pro-ESM). Raw eggshells were cleaned carefully with deionized water, and the inner membrane was manually removed from the eggshell. The obtained ESM was washed thoroughly to remove the albumin, cut into small rectangular pieces (about 5 mm × 8 mm), and then dried in vacuum at room temperature for future use. In a typical procedure, a certain amount of procyanidin was dissolved in 50.0 mL of deionized water and mixed with 0.5 g of ESM pieces prepared in the previous step. The mixture was then stirred at 298 K for 2 h. Afterward, 0.5 mL of glutaraldehyde (used as cross-linking agent between ESM and procyanidin) was added into the mixture at pH 6.5, and the mixture was stirred at 310 K for 6 h. Finally, the product was collected with forceps, fully washed with water to remove the adsorbed procyanidin, and dried in vacuum to obtain the Pro-ESM. Preparation of [email protected]
Grafted Eggshell Membrane Composites ([email protected]
). The synthesis of supported AgNPs on Pro-ESM was ascribed to the chelating and in situ reducing capacity of procyanidin toward Ag ions. The as-prepared Pro-ESM pieces were incubated with 50 mL of AgNO3 aqueous solution (10 mM) for 12 h under constant stirring at 310 K. Meanwhile, the color of ProESM changed to light brown, indicating the formation of AgNPs on the 4639
dx.doi.org/10.1021/am500665p | ACS Appl. Mater. Interfaces 2014, 6, 4638−4649
ACS Applied Materials & Interfaces
surface of the protein ﬁbers. Afterward, the resulting [email protected]
composites were again thoroughly rinsed and dried in vacuum for further analysis. Catalytic Reduction of 4-NP. To investigate the catalytic eﬃciency and reusability of the [email protected]
composites, reduction of 4-NP was performed according to our previously reported procedure.19 In a typical experiment, 15 mg of [email protected]
composites was added into a mixed solution containing 7 mL of deionized water and 750 μL of 4-NP (3 mM). N2 gas was then purged through the solution for 10 min to remove the dissolved O2. Subsequently, 1 mL of freshly prepared NaBH4 solution (0.3 M) was injected under continuous stirring to initiate the reduction reaction. At each time interval, part of the mixture was transferred into a quartz cuvette, and UV−vis absorption spectra were recorded in the range 250−550 nm to monitor the catalytic reaction. The product of the catalytic reduction was also analyzed by an Agilent 1200 HPLC system using an Agilent Eclipse XDB-C18 column (150 mm × 4.6 mm, 5 μm particle size). The reaction was conducted at four temperature levels, i.e., 303.15, 308.15, 313.15, and 318.15 K, using a temperature-controlled water bath to study the eﬀect of temperature on the catalytic property. For comparison, the control experiment was also carried out under the same experimental conditions using Pro-ESM as catalyst. The catalytic activity of the as-prepared [email protected]
composites for the reduction of other nitrobenzenes (2-nitrophenol and 4-nitroaniline) was investigated. Characterization. The growth process of AgNPs using procyanidin as reductant and stabilizer in the aqueous solution was monitored by a TU-1810 (Persee, China) UV−vis spectrophotometer. The ultraviolet− visible diﬀuse reﬂectance spectra (UV−vis DRS) of the as-prepared [email protected]
composites were recorded using a Lambda 750 Perkin-Elmer UV−vis spectrophotometer equipped with an integrating sphere using BaSO4 as reference. The morphological features were observed by scanning electron microscope (SEM, Hitachi S-4800) coupled with energy-dispersive X-ray spectroscopy (EDX) at an accelerating voltage of 3.0 kV. The detailed morphology and size distribution of the AgNPs were determined using a high resolution transmission electron microscope (HRTEM, JEM-2100F, 200 kV) equipped with an energy-dispersive X-ray (EDX) analysis attachment. After ultrasonication of the [email protected]
composites in deionized water, a drop containing the released AgNPs was deposited onto the carbon-coated copper grids and dried at room temperature for the analysis of supported AgNPs. X-ray diﬀraction (XRD) measurement was carried out using D/max 2500 XRD spectrometer (Rigaku) with a Cu Kα X-ray source. X-ray photoelectron spectra (XPS, PHI-5300 ESCA, USA) of the ESM, Pro-ESM, and [email protected]
were recorded with an Al Kα source (hν = 1486.6 eV). Peaks from all of the high-resolution core spectra were ﬁtted with XPSPEAK 4.1 software, using mixed Gaussian−Lorentzian functions. Fourier transform infrared spectroscopy (FTIR, Nicolet Nexus 670) analyses were identiﬁed within the range 400−4000 cm−1. Thermogravimetric analysis (TGA) was performed using a simultaneous TGA−DTA apparatus (PTC-10A, Rigaku, Japan), from room temperature to 700 °C at a heating rate of 10 °C/min in air. The amount of AgNPs on Pro-ESM was accurately determined by inductively coupled plasma mass spectrometry (ICP-MS, Agilent 7700x, USA) after the composites were dissolved and diluted in nitric acid.
Figure 1. UV−vis absorption spectra of AgNPs synthesized in the aqueous solution at diﬀerent times using procyanidin (0.5 mM).
signiﬁcantly red-shifted to 439 nm after 12 h, which was accompanied by the narrowing of their bandwidths and the gradual increase in absorption intensity. This phenomenon indicates the growth process of AgNPs under the mild reducing capacity of procyanidin. According to previous literature,28,32 this metallic Ag+ reducing ability of plant-extracted polyphenol is attributed to the multiple hydroxyls that can chelate with the Ag+ ions and reduce the chelated Ag+ into Ag0 in situ. The inset in Figure 1 shows a curve of the maximum absorption wavelength versus the reaction time. A negligible wavelength shift was observed from 9 to 12 h, suggesting that the NP size gradually stopped increasing because of the capping eﬀect of procyanidin (TEM analysis also support this phenomenon, as shown in Figure 2 and Figure S1, Supporting Information). Therefore, a reduction reaction time of 12 h was chosen for the preparation of supported AgNPs. The SPR peak of AgNPs are inﬂuenced by their size, as well as their morphology, compositions, surface chemistry, and surrounding environment, especially for the NPs with small diameters.33 Therefore, the morphology and size distribution of AgNPs cannot be deduced simply through the SPR peak, but they should be examined further by TEM analysis. Figure 2 shows the typical TEM images of the AgNPs that were grown for 12 h and its corresponding size distribution histogram. The TEM results indicate that the formed small-sized NPs are predominantly spherical and well-dispersed without agglomeration in the aqueous solution (Figure 2a). Hence, procyanidin can reduce Ag+ to AgNPs and simultaneously serve as the stabilizing agent to prevent agglomeration because of the rigid aromatic rings of molecular backbone in procyanidin. Lattice fringes are faintly visible from the further magniﬁed HRTEM image (Figure 2b) of the AgNPs, showing the crystalline structure of AgNPs. The corresponding fast Fourier transform (FFT) pattern (Figure 2b, inset) also indicates the single crystal nature.3 More than 200 particles in several TEM images have been analyzed using the ImageJ software to determine the size distribution. As shown in Figure 2c, the AgNPs have a narrow size distribution with an average diameter of 2.19 nm. The in situ reduction and simultaneous capping ability of procyanidin may contribute to the formation of small and uniform AgNPs.34 These results clearly suggest that the introduction of grape-seed-derived procyanidin dimer provides a nontoxic approach for the formation of uniformly dispersed AgNPs with small particle size. FTIR analysis was further used to investigate the structural changes of procyanidin during the synthesis process of AgNPs.
RESULTS AND DISCUSSION Synthesis of AgNPs in Aqueous Solution Using Procyanidin. The formation of AgNPs by the reduction of AgNO3 solution with grape-seed-derived procyanidin dimer was indicated by the concomitant change in the color of the reaction mixture from transparent to light brown within 12 h. The time evolution of the UV−vis spectra during the growth of AgNPs using 0.5 mM procyanidin as reductant is shown in Figure 1. At the earlier stage of the reaction (